Seeing Is Believing: Hot Electron Based Gold Nanoplasmonic ... Seeing Is Believing: Hot Electron...
Embed Size (px)
Transcript of Seeing Is Believing: Hot Electron Based Gold Nanoplasmonic ... Seeing Is Believing: Hot Electron...
SIL ET AL . VOL. 8 ’ NO. 8 ’ 7755–7762 ’ 2014
July 29, 2014
C 2014 American Chemical Society
Seeing Is Believing: Hot Electron Based Gold Nanoplasmonic Optical Hydrogen Sensor Devika Sil,† Kyle D. Gilroy,‡ Aurelia Niaux,† Abdelaziz Boulesbaa,† Svetlana Neretina,‡ and Eric Borguet†,*
†Department of Chemistry, Temple University, Philadelphia, Pennsylvania 19122, United States and ‡College of Engineering, Temple University, Philadelphia, Pennsylvania 19122, United States
T he interaction of metal nanoparticles (NPs) with photons whose energy is resonant with the surface plasmon
leads to the generation of plasma oscilla- tions which can decay into hot electrons.1�3
This strong interaction offers the opportu- nity to couple light to drive chemical reac- tions and provides a means to generate valuable product with relatively low energy input.2 The probability of generating ther- malized, or “hot”, electrons is increased when the metal nanoparticles are much smaller than the wavelength of the incident radiation.2
Recent studies have focused on the trans- fer of hot electrons from excited metal surfaces to nearby molecular orbitals.2,3
Mukherjee et al. provided the first experi- mental evidence for the room-temperature photocatalytic dissociation of H2 on 5�30 nm gold nanoparticles using visible light.2,3 Their results demonstrated that a fraction of the hot electrons generated by the resonantly excited gold nanoparticles allowed for elec- tron transfer into the 1σu* antibonding orbi- tal of a physisorbed H2 molecule, leading to
dissociation.2,3 The requirements for this process are that (i) the Au NPs are excited resonantly, (ii) the Feshbach energy overlaps the hot electron distribution,4 (iii) the hot electrons have energy greater than 1.8 eV, (iv) the weight fraction of Au in TiO2, or SiO2, is between 0.5% and 3%,2,3 and (v) the nano- particles are sufficiently small (
SIL ET AL . VOL. 8 ’ NO. 8 ’ 7755–7762 ’ 2014
scheme using the localized surface plasmon resonance (LSPR) was reported.17�23 The LSPR is a sensitive probe of changes in the local environment, such as perturba- tions in the dielectric properties of the medium. The collective oscillations of free electrons are driven by the interaction of plasmonic metallic nanoparticles (typically Au, Ag, or Cu) with visible light.24 Indirect nanoplasmonic sensing schemes employ an enhanced electric field to sense changes in the dielectric envi- ronment triggered by a secondary activematerial, such as Pd. When placed in the near-field of resonantly excited Au nanoparticles, an external analyte molecule (e.g., H2) changes the dielectric properties of Pd, which in turn shifts the LSPR of the Au nanoparticles.17�23 Pd was chosen due to its well-established ability to dis- sociate and absorb hydrogen and undergo a reversible lattice expansion.25,26 As shown by Liu et al., as the Pd NP approaches the near-field of a resonantly excited Au nanotriangle, the spectral position and scattering intensity of the Au system shift upon hydrogen ex- posure due to the formation of Pd hydride, which has different dielectric properties compared to Pd.22 Lan- ghammer et al. used substrate-based Au nanodisks separated from Pd nanoparticles by a thin dielectric spacer layer to study hydriding and dehydriding kinetics of 1.8�5.4 nm Pd nanoparticles.23 However, Liu et al. and Langhammer et al. did not report any hydrogen sensingwith the Au nanostructures alone.22,23
The discovery of the hot electron induced photocatalytic activity of Au nanoparticles by Mukherjee et al.2,3 shows that the Au LSPR could drive the dissociation of H2 without the need for an adjacent active material such as Pd. However, any change in the optical response of the Au nanoparticles due to hot electron induced dis- sociation of hydrogen has yet to be reported. The interaction of Au with hydrogen, especially the
formation of Au�H bonds, is far from being under- stood due to the inert nature of bulk Au. However, there are studies, both theoretical and experimental, that discuss the adsorption of hydrogen onto Au27�30
and the formation of AuHx. 30�37 Bus et al. reported that
small gold nanoparticles (∼1.4 nm) supported on alu- mina dissociatively adsorb hydrogen.30 This is accom- panied by a change in electronic properties, as it was shownbyX-ray absorptionnear-edge spectroscopy that the L3,2 edges of Au/Al2O3 recorded in hydrogen under- go a shift of several electronvolts.30 Previous reports also mentioned that the formation of surface-based AuH2
and AuH4 � is stabilized by relativistic effects38 and is
likely to occur in electron-rich systems such as provided by laser ablation and plasmas.34 The catalytic activity was associated with atomic sites of lower coordination (i.e., at the edges and corners). In this work, we optically detect the dissociation of
H2 on Au nanoparticles. The novelty stems from the room-temperature optical detection of hydrogen using (i) thermally self-assembled substrate-based
gold nanohemispheres (Au NHs) and (ii) surfactant- free structures (allowing for close contact between the nanostructures and the analyte). It is important to note that the observation of hot electron generation for spherical, larger nanostructures (>20 nm) was pre- viously reported to be negligible2,4,39 and that the dissociation of H2 was negligible.
2,4,40,41 On the con- trary, in the present study, a∼1�2% change in optical transmission was achieved at room temperature using Au NHs between 10 and 50 nm in diameter upon inco- herent excitation. To substantiate the claim of AuHx formation, discrete dipole approximation (DDA) simu- lationswere carried out using dielectric constants of Au hydride previously measured by Giangregorio et al.34
Characterization of Films. Tapping mode atomic force microscope (AFM) images of the Au NHs film (Figure 1a) showed a broad distribution of closely spaced hemispherical particles between 10 and 50 nm. A histogram is shown in Figure 1b, where the average size was measured to be∼28( 8 nm. The UV/ vis extinction spectrum (Figure 1c) showed the plas- mon band of Au NHs as a wide inhomogeneously broadened feature at ∼570 nm. The peak position appeared to be red-shifted by about 50 nm from the previously reported position of plasmon band for spherical Au NPs.42 This shift in spectral position of the plasmon band could be attributed to two effects: (a) nanoparticle shape induced effects and (b) nano- particle size related changes in surface plasmon reso- nance. The geometry-induced shift was observed previously for other metals43 and was attributed to the effective dipole being closer to the substrate. It was found that hemispheres have a stronger interaction with the substrate as compared to spheres.43,44 Nano- particle dimension induced changes in the surface plasmon resonance arise due to increased electromag- netic retardation in larger nanoparticles.45,46 In the present case, the red shift could be a cumulative result of the two aforementioned phenomena.
Plasmonic Sensing Results. The broadband incoherent excitation was selected to cover wavelengths between 500�600 nm and the real time response of the Au film (Figure 2a�c) in H2 wasmonitored. An average increase of∼1.8% in the transmitted intensity through an Au NH film, supported on a glass slide, was observed within 0.3�1 s of turning onH2. TheAuNH filmwas exposed to 10% H2 in N2 for 10�20 s, during which time the transmitted intensity stayed constant. Upon turning off the H2 flow, the transmitted intensity recovered to the initial value. Thus, from the real-time monitoring of the response of Au NHs to H2 (Figure 2), it became evident that these nanostructures act as rapid and reusable optical H2 sensors upon resonant excitation at the SPR. Details regarding the experimental setup are provided in the Supporting Information (SI, Figure S1).
SIL ET AL . VOL. 8 ’ NO. 8 ’ 7755–7762 ’ 2014
Hydriding and Dehydriding of Au NHs with UV/Vis Spectros- copy. The surface plasmon resonance of Au NHs films was tracked with and without hydrogen exposure by recording transmission spectra with a UV/vis spectro- meter. In the absence of hydrogen the signal stayed stable at a transmittance of ∼46%. Upon introducing hydrogen, a ∼1% increase in transmittance was
observed (Figure 3). After stopping H2 and waiting, the transmittance signal recovered to the initial value. The presence of hydrogen induced a blue shift of ∼3 nm.
Wavelength Dependence. Combinations of filters were placed in the beam path to vary the incident excita- tion wavelength range (See Figure S4 in SI for details) in order to study how it affected the magnitude of the optical response of the Au NH films to hydro- gen. The experiments were carried out at 293 K and under similar illumination intensities covering photon wavelengths from 400�800 nm. The change in transmission was greatest for wavelengths within 30 nm of the LSPR (λex = 550 and 580 nm) (Figure 4).
Figure 2. Real-time monitoring of changes in transmitted intensity for multiple cycles of H2. Each point plotted is the percentage change in transmitted intensity between 500 and 600 nm as a function of time. Each time increment was 0.3 s apart. Rapid response after (a) seven cycles of hydrogen, (b) 11 cycles of hydrogen, and (c) one cycle of hydrogen close up to show both the ON and OFF response.
Figure 3. Tracking the surface plasmon resonance of Au NHs in H2 with a UV/vis spectrometer. Red spectrum is without any